Discussion Chain ID: 86026
================================================================================

User asked: Is there a way to "electroplate" wood with copper?

Maybe wood can be coated with copper (II) sulphate first, or roasted in order to form a conductive charcoal (carbon) layer.

Discussion:
Comment: Galvanising usually means coating with zinc. But the short answer is: it would be very difficult to coat wood with copper metal.
Comment: @Gert Didn't know that, i am not a native speaker of english. I corrected for "electroplate".
Comment: *Electroplate* implies the substrate has some electrical conductivity. Wood's is very poor, hence the difficulty.
Comment: @Gert It's difficult indeed, hence the question.
Comment: I like the concept of roasting the wood, but I don’t see how you would get a uniformly conductive surface due to the organic structure of the wood. If you coated it with copper sulfate, you would end up losing your conductive layer as it the sulfate salt would likely dissolve in your electrolyte as soon as you put it in. That’s why algae resistant paints used on boats need a sacrificial anode to be effective.

Answer 1 (16 votes):
The most common way to apply metals by electrodeposition to nonconductive materials is to apply a "strike" of underlying metal, usually nickel or copper, via a method like [electroless plating](https://en.wikipedia.org/wiki/Electroless_plating). In electroless, the electrons for the reduction of the metal ions to the zero-valent state are supplied by a reducing agent in solution: $$ \begin{align} \ce{Red &-> Ox + 2 e^-} \\\ \\\ \ce{Ni^{2+} + 2 e^- &-> Ni^0} \end{align} $$ This "strike" coating is then used to provide the electrical connection necessary to apply the metal of interest—here, copper—by typical galvanic electrodeposition methods.

Discussion on this answer:
Comment: This solution came to my mind, but would this "strike" actually hold on to the wood?
Comment: @Mithoron As long as the wood was dry and in good condition (not crumbling, rotting, etc.), I would expect the strike to hold quite well, actually. You'd want to use seasoned wood to minimize swelling/shrinking, and you'd have to have the wood submerged for the absolute minimum time possible, but I think it has a decent chance of working. The porosity and texture of the surface should be well suited to it. Of course, there could easily be complications I'm not anticipating.

Answer 2 (8 votes):
Dip the wood in a solution of ascorbic acid (Vitamin C; orange juice will do) and soap and allow it to soak. Soaking time will vary by wood variant. then dip the wood in a solution of copper sulfate or another copper salt and soap. The ascorbic acid will reduce the copper, creating a conductive coating. This may need to be repeated to achieve a continuous conductive coating. Finally, rinse and dry and you are all set.

Discussion on this answer:
Comment: Homemade electroless, nice! What does the soap do?
Comment: Has this been done before?
Comment: have you tried this? I would be amazed if orange juice has sufficient ascorbic acid to pull this off, and it has loads of stuff you don't need or want. In the UK you can buy a big tub of ascorbic acid powder from Holland and Barret health foods extremely cheaply. There used to be one called Linus Brand and Boots drugstores also used to do it. I know vitamins are far more difficult to come by in Spain, for example, where I have only seen them in licensed pharmacies.
Comment: I've done it on glass with pure ascorbic acid.
Comment: @A.K. I tried this, and it dit not work. I used solutions from tap water which were about saturated (some grains still visible in the vessel) at room temperature. I then dipped pices of beech wood, oak and balsa wood, dried them over night, and then dipped them into the other vessel, over several rounds. I left them in the bath for hours, until the weight hinted that the were fully soaked (it was small pieces). No effect thought. Just a light green colour, which also is what get if you mix the solutions directly.
Comment: @A.K. I got the same result that HannesH did. The soap I used was Fels-Naptha , a true soap, not a detergent. The Fels-Naptha gave a pH of about 9 or 10, a good sign as the ascorbic acid reaction proceeds in a basic, not acid solution. Further complicating things was that the copper sulfate/soap solution gave a flocculant. What "soap" did you use? What was the pH of the ascorbic acid/soap solution? Further details would be greatly appreciated.

Answer 3 (3 votes):
Using [Marble's Reagent](http://www.metallographic.com/Etchants/Etchants.htm) to etch stainless steel, the wood stirrer got coated with copper. Marble's is $\ce{CuSO4}$, $\ce{HCl}$ and water, but I think I added extra $\ce{CuSO4}$. This isn't technically electroplating, though.

Discussion on this answer:
Comment: So that is a mix of hydrochloric acid and copper sulphate? I wonder if the process here is that the wood undergoes hydrolysis from the acid, forming charcoal, which then is a reductand to the copper sulphate.

Answer 4 (2 votes):
It might be possible to evaporate the copper in a vacuum so that it is deposited on the wood. No electric conductivity required. Here is an example using gold. [YouTube: Gold & Casio Watch - Periodic Table of Videos](https://www.youtube.com/watch?v=7dF0QTzcuac) And a search found this random document about it [random document about vacuum evaporation](http://users.wfu.edu/ucerkb/Nan242/L06-Vacuum_Evaporation.pdf)

Discussion on this answer:
Comment: The question asks specifically about _electro_ plating.
Comment: @pipe since wood is non-conductive, some way to coat wood with something conductive is a requirement for electroplating, and thus well within my question.
Comment: The word electroplate in the question is in quotes which I interpreted to mean "not necessarily literal electroplating".

Answer 5 (0 votes):
Take finely powdered graphene and mix in a water based Polyurethane. Put a copper nail (or drill a hole and epoxy a wire) into the wood in an inconspicuous area to be plated. Paint a very light coating over the surface ensuring that you have surrounded the nail (or wire) and make sure the section you want plated has a uniform coating of graphene. You should be able to plate on this now conductive piece of wood. Alternatively, there are conductive silver-based paints, but these are relatively expensive. You’re going to have to figure out a way to weight this down to keep it submerged in the electrolyte because it’s going to want to float.


================================================================================

